This article was originally published in a journal published byDocument Transcript
This article was originally published in a journal published by Elsevier, and the attached copy is provided by Elsevier for the author’s beneﬁt and for the beneﬁt of the author’s institution, for non-commercial research and educational use including withoutlimitation use in instruction at your institution, sending it to speciﬁccolleagues that you know, and providing a copy to your institution’s administrator. All other uses, reproduction and distribution, including withoutlimitation commercial reprints, selling or licensing copies or access, or posting on open internet sites, your personal or institution’s website or repository, are prohibited. For exceptions, permission may be sought for such use through Elsevier’s permissions site at: http://www.elsevier.com/locate/permissionusematerial
Dent Clin N Am 51 (2007) 359–378 Aesthetic Anterior Composite py Restorations: A Guide to Direct Placement co Brian P. LeSage, DDSa,b,c,* a Beverly Hills Institute of Dental Esthetics, CA, USA b UCLA Aesthetic Continuum, CA, USA c Department of Restorative Dentistry, UCLA Dental School, CA, USA al on Mastering anterior direct composite restorations is a necessity for thecontemporary clinician who appreciates and understands the art and scienceof cosmetic dentistry. In the esthetic zone, composite bonding procedures rsare considered the most conservative and least invasive technique to returnmissing, diseased, and unsightly tooth structure to enhanced color, form,and function. The attractiveness and popularity of composites are easy to peexplain because these restorations have excellent esthetic potential, verygood to excellent prognosis, and a reasonable fee [1,2]. Composites are the most versatile restorative material available to thedental professional, especially for the esthetic-conscious patients. Therestorative dentist can use this versatile material in a mirage of indications rsand techniques. It is used as a direct and indirect restorative material on an-terior and posterior teeth, orthodontics attachments and bracket cement, in-direct restoration cements, correction of erosive and abfraction lesions, obases, liners, core build-ups and post and cores, mock-up for anterior es-thetic or posterior occlusal trial therapy, splinting, provisionalization, gingi- thval stabilization, and so forth. For composite restorations to mimic natural tooth structure, the clinician Aumust have a comprehensive understanding of the material science andtechniques involved in direct bonding procedures. Material science can bebroken down to include types of composites, tints, opaquers, adhesivesystems, and armamentarium. The necessary techniques involve an under-standing of color, adhesive principles, layering to create polychromicity,incisal eﬀects and perfect imperfections, and ﬁnishing and polishing. * 436 North Roxbury Drive, Suite 100, Beverly Hills, CA 90210. E-mail address: firstname.lastname@example.org/07/$ - see front matter Ó 2007 Elsevier Inc. All rights reserved.doi:10.1016/j.cden.2007.02.001 dental.theclinics.com
360 LESAGEComposite materialsComposition A composite is a multiphase substance formed from a combination ofmaterials that diﬀer in composition or form, remain bonded together,and retain their identities and properties . They have four main com- pyponents: (1) resin (organic polymer matrix); (2) ﬁller (inorganic) parti-cles; (3) coupling agent (silane); and (4) the initiator-accelerator ofpolymerization. coResin matrix Manufacturers prefer Bis-GMA resins because they have an aromaticstructure that increases stiﬀness and compressive strength and lowers alwater absorption . Bis-GMA 2,2-bis [4(2-hydroxy-3 methacryloyloxy-propyloxy)-phenyl] propane is the most popular dimethacrylate resin, but to onaccommodate better ﬁller load triethylene glycol dimethacrylate or urethanedimethacrylate is added . rsFillers Filler (inorganic) particles provide dimensional stability to the soft resin pematrix . The ﬁller particles used in composites vary in size from less than0.04 u to over 100 u. Common ﬁllers are crystalline quartz; colloidal and py-rolytic silica; and such glasses as lithium, barium, or strontium silicate.Coupling agent rs Silane helps form a good bond between the resin matrix and ﬁller parti-cles during setting. The silane contains functional groups (eg, methoxy) that ohydrolyze and react with the inorganic ﬁller, and unsaturated organicgroups that react with the resin matrix during polymerization . thInitiators and accelerators of polymerization Au Composites contain initiators and accelerators that allow for light-, self-,and dual-cure modes. For visible light activation, camphoroquinones(0.03%–0.09%) start the free radical reaction using blue light in the468 nm Æ 20 nm range . In the esthetic zone, light-cured compositesare the material of choice because color matching and color stability arethe most predictable. For chemical-cured composites, aromatic tertiary amine (2%) initiatesthe free radical reaction when the paste and catalyst are mixed. Tertiaryamines (and HEMA found in many adhesive systems) have been found tocause color change in composites on polymerization .
AESTHETIC ANTERIOR COMPOSITE RESTORATIONS 361Classiﬁcation and application Historically, composites have been classiﬁed by particle size, shape, anddistribution of ﬁllers [5,6]. In the 1980s and 1990s, composite technology de-veloped and became reﬁned into two classiﬁcations: microhybrids and mi-croﬁlls. At the new millennium, nanotechnology introduced a new class of pycomposite: the nanoﬁllers. The three classiﬁcations of composites have theirvery distinct indications, advantages, and disadvantages (Table 1). An ideal composite consists of the following four qualities: (1) mirror conatural tooth structure in color and translucency; (2) strength to withstandfunction in stress-bearing areas for the long-term; (3) seamless or undetect-able margins from restoration to tooth for the long-term; and (4) achieve theappropriate contour and polish (luster and ﬁnish) and maintain it for thelong-term . alMicrohybrid on Microhybrids contain a distribution of two or more irregular-shaped, butrather uniform diameter, ‘‘glass’’ or quartz particles of 0.2 to 3 mm plus 5%to 15% 0.04-mm microﬁne particles. This distribution of ﬁllers makes the mi-crohybrid 60% to 70% ﬁlled by volume, which translates roughly into 77% rsto 84% by weight [2,3,8] (Table 2). The particle sizes and distribution and percent ﬁlled by weight lead to the pefollowing advantages for the microhybrid composite: strength; lower poly-merization shrinkage (0.6%–1.4%); lower coeﬃcient of thermal expansion;lower values of water sorption; higher ﬂexural strength; and higher Knoophardness [2,3,8]. Their disadvantage is maintaining a polish for the long-term. rsTable 1Indications, advantages, and disadvantages of the three major categories of composite resinsClassiﬁcation Indications Advantages Disadvantages oMicroHybrid Layer the desired Strength: less likely Polishability: not shade deep within the to chip in long-term th restoration to mimic high-strength area dentin and enamel Refractory properties: morphology opacity similar to Au Provide strength in any enamel and dentin functional areaMicroFill Replace enamel in color Polishability: high shine Lacks strength and translucency for the long-term for some Polish ability Wear: resistance better functional areas Wear resistance and than microhybrids Can be too surface texture Refractory properties: translucent translucency similar to enamelNanoFiller All anterior and Potential advantages of No in vivo posterior restorative MicroHybrid and long-term studies applications?? MicroFill
py co 362Table 2 alFiller sizes in the three major categories of composite resinsClassiﬁcation Size of ﬁller Volume of Filled byof composite particles (mm) inorganic ﬁller (%) weight (%) DiagramMicroHybrid 0.2–3 plus 0.04 60–70 on 77–84 rs LESAGEMicroFill 0.02–0.04 32–50 50–70 peNanoFiller 0.01–0.04 60–72 79–84 o rs th Au
AESTHETIC ANTERIOR COMPOSITE RESTORATIONS 363 From an esthetic standpoint, microhybrids have more opacity and are ex-cellent in replacing dentin. Microhybrids with smaller average particle sizesare excellent in replacing enamel and can be good to excellent in holdingtheir polish over time. Examples of contemporary microhybrids includeHerculite and Point 4 (Kerr/Sybron, Orange, California), Filtek Z250 (3MESPE, St. Paul, Minnesota), and Vitw1wescence (Ultradent Products, pyInc., South Jordan, Utah).Microﬁlls co Microﬁlls contain colloidal silica ﬁllers of 0.04-mm particle size and a ﬁllerloading of 32% to 50% by volume, which equates to 50% to 70% by weight[3,8] (see Table 2). Because microﬁlls are less highly ﬁlled, they have higher polymerizationshrinkage, coeﬃcient of thermal expansion, and water sorption compared alwith microhybrid composites. They demonstrate excellent polish and wearcharacteristics. Their disadvantage is strength and in some clinical situations onbeing too translucent. From an esthetic standpoint, microﬁlls are superior to microhybrids. Mi-croﬁlls are excellent in replacing enamel, creating translucent zones, and rshaving appropriate anatomy and high polish for the long-term. Examplesof contemporary microﬁlls include Filtek A110 (3M ESPE, St. Paul, Minne-sota), Renamel (Cosmodent, Chicago, Illinois), and Matrixx Anterior Mi- pecroﬁll (Discus Dental, Culver City, California).Nanoﬁllers Two nanoﬁllers are the aggregated zirconia-silica cluster ﬁller (3M) with rsan average cluster particle size of 0.6 to 1.4 mm with primary particle size of5 to 20 nm and a nonagglomerated-nonaggregated 20-nm silica ﬁller ; andthe Kerr prepolymerized ﬁller (30–50 mm; barium glass, 0.4 mm; and silicananoparticles, 0.02 mm). Nanoﬁllers contain zirconia-silica nanocluster oﬁllers of 30 to 50 mm (0.02 mm) plus submicron 0.01 to 0.02 mm silica parti- thcles. Nanoﬁllers exhibit ﬁller loading of 60% to 72% by volume, whichequates to 79% to 84% by weight  (see Table 2). Examples of contempo-rary nanoﬁllers include Premise (Kerr/Sybron, Orange, California), Aelite AuAesthetic Enamel (Bisco, Schaumburg, Illinois), and Filtek Supreme PlusUniversal Restorative (3M, St. Paul, Minnesota). Being relatively new, nanoﬁllers have few long-term in vivo studies, whichis their disadvantage. Some shorter-term studies exist, and empirically thisclassiﬁcation of composite has the potential to exhibit the advantages andlimit the disadvantages of the other two composite classes. Because of theirhigher volume percent loading they exhibit lower shrinkage and associatedless pull on margins, adhesives, and interproximal contact issues. More stud-ies over a longer period of time are very much needed, however, to supportsuch an opinion.
364 LESAGEAdhesive systems and techniques The success of composite restorations is directly related to the success ofthe adhesive system and technique used. Adhesive dentistry when appliedcorrectly can prevent the dislodgement of composite restorations, preventsensitivity issues, prevent microgap formation or microleakage leading to re- pycurrent decay, and so forth. In article by Dr. Perdigao, a complete and com-prehensive understanding of adhesives can be gained. coTints A tint is a color that is mixed with white. The tinted range of any one colorcan run from the pure color at its maximum intensity through to white .For the restorative dentist, a tint’s primary indication is to match natural altooth structure in polychromicity and maverick colors. It can also be usedto help mask out the tooth-restoration interface. The eﬀect on color is tolower the value. Tints are very intense colors and need to be used judiciously on(Table 3). rsOpaquers Opacity is the opposite of transparency, and describes the degree to pewhich light is prevented from passing through the color. It sometimes is de-scribed as ‘‘covering power,’’ and is the color’s ability to cover an underlyingcolor, preventing any trace of the latter showing through . The primary indication for an opaquer is to block out any size, shape,and degree of darkness within a tooth using only a thin layer of material.If the restorative dentist can create a stump shade that is uniform in poly- rschromatic color, the ﬁnal restoration need only reproduce the value andtranslucency of enamel. Opaquers can also help to block out the tooth-restorative interface and block out excessive translucency in CL III and oIV restorations. Their eﬀect on color is to raise value (see Table 3). th AuTable 3Overview of tints and opaquers IndicationsTints Match natural tooth structure in polychromicity and maverick colors Help mask out tooth-restorative interface Lower the valueOpaquers Raise the value Block dark tooth color in thin layer Help mask out tooth-restorative interface Block excessive translucency in CL III and IV restorations
AESTHETIC ANTERIOR COMPOSITE RESTORATIONS 365Layering techniquesOverview When considering the direct anterior restoration in composite, one needsonly to borrow from nature. If one studies and understands natural toothstructure in color, form, and function, then composite mirroring becomes pythe objective. Composite mirroring is the natural replacement of teethwith minimal or no additional removal of the intact, health dentition to nor-mal form and function with tooth-colored material. With this approach, the corestorative dentist must indulge the optical, anatomic, and functional char-acteristics of natural teeth. In composite mirroring, the restorative dentist chooses an enamel anddentin replacement material that emulates the missing tooth structure in op-tical properties and strength. Clinically, this can be oversimpliﬁed by using ala microhybrid in any area requiring strength or dentin replacement and a mi-croﬁll for polishability and enamel replacement and eﬀects (Fig. 1, Table 4). onFigs. 2–5 shows a more in-depth breakdown of the composite mirroring sys-tem. Nanoﬁllers, with more clinical data, may eventually eliminate the needfor both systems. When used properly, the composite mirroring system of layering is rscrucial in creating life-like restorations in strength and esthetics includingpolychromicity and incisal eﬀects. The layering of composite material can pebe simple, involving one or two shades, or advanced, mimicking the ar-tistic skills of the ceramic technician. When describing the four layeringtechnique, trying to simplify or categorize which layering technique is o rs th AuFig. 1. Simpliﬁed, generalized overview of the composite mirroring system. Brown area using mi-crohybrid for the stress-bearing zone (strength for the long-term), and beige area using a microﬁllfor esthetics (polishability for the long-term). (Courtesy of Brian LeSage, DDS, Beverly Hills, CA.)
366 LESAGETable 4Overview of tooth structure replacement and classiﬁcation of composite resinsTooth structurebeing replaced Microhybrid MicroﬁllEnamel: stress-bearing area þþþþ þ (need support of tooth)Enamel: pure esthetic area þþwþþþ þþþþ pyDentin: pure esthetic area þþþwþþþþ þþþwþþþþ (higher chroma (ie, CL III, V) needed)Dentin: stress-bearing area þþþþ þ (need support of MicroHybrid) (ie, CL IV) co Abbreviations: w, not indicated; þ, least indicated; þþþþ, highly indicated.best, the clinician needs to consider the patient’s ﬁnancial commitmentand the esthetic wants of the patient. Visualization, being able to seeand believe in creating the end point, is critical. The purpose of compos- alite layering is to establish the dentin layer and dentinal lobes in a toothand create the wonderful nuances of enamel and enamel eﬀects that ontransform into incisal translucency and incisal halo eﬀects [7,11–16,17–21].Shade selection technique rs The shade selection technique is as follows [18,22–26]: pe 1. Pumice tooth lightly to remove any stains, debris, pellicle, and so forth, but not so much as to inﬂuence the tooth’s natural luster and ﬁnish. Oth- erwise, this could aﬀect the predictability of shade matching (Fig. 6A). 2. The dentin shade is best obtained from the gingival third of the tooth where the enamel is the thinnest (Fig. 6B) or from the canines where o rs th AuFig. 2. Simple layering technique. Brown area demonstrating the use of one shaded material,and the hashed zone an optional second shaded material of diﬀerent opacities and the sameor diﬀerent chroma range. (Courtesy of Brian LeSage, DDS, Beverly Hills, CA.)
AESTHETIC ANTERIOR COMPOSITE RESTORATIONS 367 py co al onFig. 3. Less simple layering technique. Same as simple layering technique with the addition ofa translucent zone internally to help distinguish the dentinal lobes and create incisal eﬀects.(Courtesy of Brian LeSage, DDS, Beverly Hills, CA.) rs the chroma is the greatest. Clinically, this is done by placing a small thin convenience form of the anticipated shade in the gingival third and light pe curing. This must be done before the teeth dehydrate. It should be noted that microhybrids generally get darker on light curing, and microﬁlls get lighter when light cured. 3. The enamel shade is conveniently obtained in the middle third of the tooth, where the enamel is the thickest (Fig. 6C). rs 4. The incisal or translucent shade is observed in the incisal third of the tooth, where the enamel is the thickest and there is little dentin opacity. In most anterior teeth the translucent zone is not limited to the incisal edge but carries into the transitional line angle zones (Fig. 6D). o 5. Color mapping by the clinician doing the esthetic composite restoration th aids the clinician because these procedures can be lengthy and often the operator’s eyes fatigue physically and mentally. The color map is a pic- ture or prescription to be used as a guide throughout the fabrication of Au the direct restoration (Fig. 6E). 6. Practice mock-up using the selected shades can be done quickly with- out good adhesive technique to act as a shade evaluation guide and subsequently to fabricate a putty matrix. Once one is satisﬁed with the color based on the mock-up, the clinician turns their attention to contour. Modify the mock-up to obtain the correct outline form, embrasure form, incisal edge, and incisal plane contour to the facial- incisal line angle (do not spend time getting the facial surface ideal at this point). At the same time, get the centric stops and anterior dis- clusion that is needed for longevity. Once the occlusion and contours
368 LESAGE py co alFig. 4. 3-D Advanced Layering Technique. Brown area demonstrating the use of TWO opa- oncious shaded materials varying in chroma (D2-Higher Chroma Dentin opacious shade, D1-Lower Chroma Dentin opacious shade) and a translucent zone (T) internally to help distinguishthe dentinal lobes and additionally an outer layer of enamel material (E) of the same or diﬀerentchroma range. Lingual hashed enamel layer can be the E shade or the D2 shade. (Courtesy of rsBrian LeSage, DDS, Beverly Hills, CA.) are correct, use a stiﬀ VPS material, such as Aquasil Ultra Rigid pe (Dentsply/Caulk), Aﬃnity (Clinician’s Choice), Imprint II (3M ESPE), and Exaimplant (GC), to fabricate a putty matrix that cap- tures the entire lingual contour completely to the facial-incisal line an- gle  (Fig. 6F, G, and H). rsSimple layering technique This technique should be considered for the patient who has minimal es-thetic concerns, but when all decisions are based on economics. One or two oshaded materials (with diﬀerent opacities and the same or diﬀerent chroma thrange) suﬃce (see Fig. 2).Less simple layering technique Au This technique should be considered for the patient who has moderateesthetic concerns, but when decisions are based primarily on economics. Itentails one or two shaded materials (with diﬀerent opacities and the sameor diﬀerent chroma range) and another layer using incisal shaded material(Fig. 3).Three-dimensional advanced layering technique This technique should be considered for the patient who has a moderateto extensive understanding of esthetics and when ﬁnances play minimally
AESTHETIC ANTERIOR COMPOSITE RESTORATIONS 369 py co al on rs peFig. 5. (A) 3-D Characterized Layering Technique. Same as 3-D Advanced Layering techniquewith the lingual enamel layer being a distinct (E) layer. And the addition of a second facialenamel layer of diﬀering chroma range to internally give depth to the dentinal lobes and createincisal eﬀects mirroring mother nature. Not shown is the tint layer placed internally creatingmaverick colors and eﬀects. (B) Sequential application and layering starting from the lingual rsand extending to the facial with multiple dentin and enamel shades, and a translucent shade.(Courtesy of Brian LeSage, DDS, Beverly Hills, CA.) ointo their decision-making process. Two shaded materials with diﬀerent thchromas are used to replace dentin, with an enamel layer for enamel eﬀectsand another layer using incisal shaded material (Fig. 4). AuThree-dimensional characterized layering techniques This technique should be considered for the patient who has a very highesthetic intelligence quotient and is very esthetically demanding, and whenﬁnances are not part of their decision-making process. Two shaded mate-rials with diﬀerent chromas are used to replace dentin, two shaded materialswith diﬀerent chromas are used for the enamel layer for enamel eﬀects, andanother layer uses incisal shaded material. A characterization layer is placedbetween the incisal and enamel layers or the two enamel layers depending onthe intensity of the eﬀect desired (Fig. 5). Tints are placed internally to
370 LESAGE py co al on rs pe o rs thFig. 6. Shade Selection Technique. (A) Before picture at 1:1 showing worn and chipped areasafter lightly pumicing. (B) Highlighted gingival 1/3 for dentin shade selection. (C) Highlighted Aumiddle 1/3 for enamel shade selection. (D) Highlighted incisal 1/3 for translucent shade selection.(E) Color mapping to aid in shade predictability. (F) Mock-up used for preliminary shade deter-mination and 3-D spatial relations to fabricate putty matrix. (G) Putty Matrix trimmed properlyto the facial incisal line angle. Note bevel and star burst bevel. (H) Final restoration appearingseamless and mirroring mother nature. (Courtesy of Brian LeSage, DDS, Beverly Hills, CA.)mirror the unique characterizations of the natural tooth, such as subsurfacestaining or demarcations of any color, shape, or size. The outer layer is unique and preplanned in this technique. If the desiredoutcome is a brighter (higher value) shaded tooth, then the outer layer musthave enamel color. Enamel shade should be used a the outer layer and the
AESTHETIC ANTERIOR COMPOSITE RESTORATIONS 371 py co al on Fig. 6 (continued) rs peincisal shade internally. If the ﬁnal outcome desired is a tooth with lower value,then the outer layer is the translucent shade, which on top of the last enamelshade acts as a transparent ﬁltering layer resulting in a lower value. As the complexity of the layering technique occurs, it is important toevaluate each layer from the incisal view and sagittal view. The clinician rsneeds to be aware if they are in the dentin substitute zone or enamel substi-tute zone. If the various layers are added too thick, all additional layers aretoo far facial and removed in the contour and ﬁnishing phase. o thSeamless margins The purpose of composite layering is to establish the dentin layer and den- Autinal lobes in a tooth and create the wonderful nuances of enamel and enameleﬀects that transform into incisal translucency and incisal halo eﬀects. Ifthese layers have voids or are not seamless, breakdown of the restorationor the tooth restoration interface is detected early. Listed are multiple stepsthat must be followed to created undetectable margins [7,20,28,29]: 1. Place a proper bevel. a. Facially on enamel: 2-mm knife-edge type. An additional starburst bevel with varying depths and lengths is an added beneﬁt. These mul- tiple bevels extend from the cavosurface margin outward, some re- maining only in enamel and others depths involving dentin (Fig. 7).
372 LESAGE py coFig. 7. Typical 2 mm long knife-edge bevel from mesial to distal; white line shows variability indepth and length of starburst design on mesial half of incisal edge. (Courtesy of Brian LeSage,DDS, Beverly Hills, CA.) al b. Facially on dentin: no bevel, butt margin. c. Lingually on enamel: chamfer margin preferably not in the contact zone. on 2. Etch past the end of the bevel. By etching past the enamel bevel, the cli- nician is able to ﬁnish the composite to inﬁnity slightly past the end of the bevel. This technique makes for a disappearing margin and allows rs for further longevity of the restoration because future polishing becomes necessary in the maintenance phase. pe 3. Roll the outer layer with clean gloved hands for sculptability and to pre- vent inclusions or voids. Once the convenience form of the desired shade of material is removed from the composite container, it has a cut or white chalky nature to the edge. If used right out of the container this zone may show up as a void in the ﬁnal restoration. By taking the allo- rs cated amount of material and rolling it in clean gloved hands one can accomplish two important roles: the material is warmed slightly and is now in a better sculptable state, and the cut portion is not detectable be- cause it is one uniform mass. o 4. Sculpt the outer layer and get the geometric outline form, transition line th angles, and primary anatomy to approximately 85% before curing. This can involve leaving the interproximal matrix (Mylar plastic strips; Com- posi-Tight metal matrix, Garrison Dental Solutions; Palodent metal Au matrix, Dentsply/Caulk) in place or removing it by pulling toward the lingual and using composite instruments and brushes to contour before light curing. 5. Super cure the composite and wait 10 minutes before ﬁnishing. Because composites cannot be overcured and the conversion is never 100%, it is best to super cure to maximize the physical properties of the material. The material continues to cure even after the light is removed; give the material time to relax before ﬁnishing. 6. Finish the margin back to between the etch and the end of the bevel. As described in step 1, the composite should be ﬁnished out to inﬁnity. By
AESTHETIC ANTERIOR COMPOSITE RESTORATIONS 373 ending this margin slightly past the bevel, as the margins pick up stain over time there is a very thin zone of material that still remains polish- able and easy to maintain. 7. Rotate ﬁnishing armamentarium from restoration to tooth. When using rubber or silicone ﬁnishing discs embedded with silicon carbide, alumi- num oxide (degrees of grit) to prevent the grit from embedding in the py margin, have the disc spinning from restoration to tooth. 8. Do not use rubber on the margins. Many manufacturers have excellent rubber polishing systems. These are best used in the body of the resto- co ration and not at the margins because the rubber shavings can get em- bedded in the margin. 9. High polish appropriate for the natural dentition. An appropriate polish and luster is the key that maintains itself for the long-term (see section on polish and ﬁnishing). al onCustomizationOverview rs In the composite mirroring layering technique, the ultimate result was ob-tained by using four to ﬁve diﬀerent shaded or translucent materials witha very particular objective in mind. Tints were also mentioned, but the tech- penique or application is now described. There are ﬁve easily learned techniques to mirror the natural dentition incheck lines, spots, craze lines, and any other maverick color issues seen innature. It must be noted that tints are very strong, and while performingthe layering technique many times the tints tend to disappear. They reappear rsas the polishing sequence progresses. Tints must never be placed on the sur-face, because ﬁnishing and polishing lead to their removal. Tints can bemixed to create a unique, desired color. The ﬁve techniques to creating a nat- oural craze line are as follows: th 1. Paint and thin: Using a thin paintbrush with the desired tint, usually white or brown, place the tint to mirror the adjacent tooth. The tint is on the tooth but way too wide and so thin the material from both Au sides leaves a thin, nonstraight line. Then light cure. 2. Scar and paint: Scar or scribe the tooth with a thin metal disc (VisionFlex, Brasseler, Savannah, Georgia) or diamond bur. Paint the desired colored tint in the scribed area and clean the excess. Then light cure (Fig. 8). 3. Matrix: After placing the second-to-most outer layer and before curing, place a Mylar or metal matrix into the composite, preferably non- straight, and light cure. Remove the matrix, paint the desired colored tint in the grooved area, and clean the excess. Then light cure. 4. Vertical wall for depth: While placing the second-to-most outer layer create a wall in the composite, preferably nonstraight, and light cure.
374 LESAGE py coFig. 8. (A) Tint application internally showing lines and dot maverick colors in second-to-lastlayer. (B) The ﬁnal restoration. (Courtesy of Brian LeSage, DDS, Beverly Hills, CA.) Paint the desired colored tint on the walled area and clean the excess. Then light cure. al 5. Anneal material over the tint: While placing the most outer enamel or dentin layer create a notch or groove in the composite, preferably non- straight. Paint the desired colored tint in the notched or grooved area on and anneal the composite toward and within itself, preferably in a non- straight pattern. Then light cure. rs These techniques are best to learn on extracted teeth or typodont teeth,where the skills can be perfected in a nonclinical setting. Habituation isneeded to master any new technique. peFinishing and polishing This is considered by many to be the most diﬃcult phase of anterior com- rsposite restorations. If the clinician follows the described guidelines of thisarticle, this step becomes routine and not one to be feared. Finishing andpolishing is crucial in ﬁnalizing the composite restoration to mimic naturein form, function, and longevity . o There is no shortcut in fabricating life-like restorations. Properly ﬁnished thand polished composites allow for a proper seal of the restoration, which in-ﬂuences its durability and allows for minimal stain accumulation, less pla-que accumulation, and better wear resistance and marginal integrity Au[28,29,31,32]. The ﬁnishing sequence includes diamond burs, followed bypolishing discs or rubber polishing discs, points, wheels, and polishingwith buﬃng wheels and polishing paste. Diamonds burs, speciﬁcally submicron diamonds of 50 mm or less UCLALeSage Anterior Preparation Bur System (Brasseler USA, Savannah, Geor-gia), run with copious amounts of water are used to create and modify therestoration to the proper geometric outline form and contours, including theproper line angles and primary and some secondary anatomy . As seen inFig. 9, blue articulating paper can help guide the clinician through thisprocess. In conjunction, course and ﬁne polishing disc (KerrHawe, Kerr,
AESTHETIC ANTERIOR COMPOSITE RESTORATIONS 375Orange, CA; EP Polishers, Brasseler, Savannah, GA; Sof-Flex Disc, 3M, St.Paul, MN; Flexi-discs, Cosmodent, Chicago, IL) run with copious amountsof water can be used to get to hard-to-reach areas to reﬁne the aforemen-tioned anatomic landmarks. Many times the loss of secondary anatomy isseen after this step. With the aid of electric handpieces (Ti-Max NL 400,NSK, Brasseler, Savannah, Georgia) and diamond burs, the clinician can pyre-establish the primary and secondary anatomy. One should check for sta-ble centric stops and appropriate anterior disclusion. The ﬁnishing phase isnot complete until interproximally and gingivally no overhangs remain and cothe geometric outline form is complete. Gingivally, the use of hand instrumentation may be more ideal to removeﬂashing or potential overhanging material. Bard-Parker #12 or #15 bladesare probably most popular, but carbide composite carvers are consideredequally eﬀective. The carbide carvers (Brasseler, Savannah, Georgia) come alin several shapes matching closely to the gingival area of intended use. Interproximally, the use of metal ﬁnishing strip (VisionFlex Strips, Brass- oneler, Savannah, GA, GC International Metal Strips, GC America, Alsip, IL)will initiate the bulk reduction. To make appropriate embrasures, the use ofan interproximal diamond disc is needed. Embrasures need to be deﬁned bydepth and volume, and the best way to accomplish this is with thin diamond rsdiscs (VisionFlex Disc, Brasseler, Savannah, Georgia) on a straight or con-tra-angle. Completing the ﬁnishing and polishing of the interproximal and petransition zones is crucial, because these areas are more prone to stainand plaque accumulation. The use of plastic interproximal strips (Sof-LexStrips, 3M, St. Paul, MN; Vivadent Strips, Vident, Brea, CA) of two gritsis essential to attain the ideal polished surface in this stain-susceptible zone. Texture creation is the tertiary anatomy that makes an average composite rsrestoration become life-like. Several possible techniques to consider are o th AuFig. 9. Technique showing the use of articulating paper to mirror primary and secondaryanatomy. (A) Once primary anatomy is close, smudge articulating paper across entire surfaceof tooth; note ﬂatness and no facial anatomy or texture in facial veneer restoration on tooth#9. (B) Articulating paper conﬁrming primary, secondary, and tertiary anatomy in direct com-posite restoration mirroring that of adjacent tooth #8. (Courtesy of Brian LeSage, DDS, BeverlyHills, CA.)
376 LESAGEtapping or dragging a course or medium diamond bur or disc with an air orelectric handpiece, using the corner or side of a cross-cut ﬁssure bur, or us-ing a white or green stone with various motions. This completes the ﬁnishingphase. All that is left is to establish the appropriate polish and luster. To obtain the appropriate high polish the use of chammy-type buﬃngwheels and discs (Flex-Buﬀ Disc, Cosmedent; Chammy wheel, Brasseler, Sa- pyvannah, Georgia) on contra-angle and straight slow-speed handpiece is re-quired. The use of a polishing paste (Luster Paste, Kerr, Orange, CA;Enamelize, Cosmodent, Chicago, IL; Truluster, Brasseler, Savannah, GA; coor Prisma-Gloss, Dentsply/Caulk, Milford, DE) wet then dry will add glossto the ﬁnal restoration. Created is a composite restoration that not only mimics the beauty ofdentin and enamel, but also deﬁes detection. There are still two remainingsteps to consider. The ﬁrst is to clean, etch, rinse, and place a seal or glaze al(BisCover LV, Bisco) on the restoration to seal any microcracks or micro-surface defects from staining. The second is to take photos for self-evalua- ontion and return of the patient with in 5 days (prescheduled) to make anyalterations detected in the photography and modify any occlusal contacts,especially in anterior guidance movements. rsSummary pe Taking a systematic approach to direct composite restorations cangreatly enhance the outcome of this multifaceted discipline. To enjoy thetrue art and science of cosmetic dentistry, the clinician must have a thoroughunderstanding of tooth morphology and topography; tooth shade analysis;composite systems and layering techniques; and the use of tints, opaquers, rsand maverick colors and zones to create restorations that mimic nature.Once the diseased, missing, or unsightly tooth structure has the exquisitebeauty of enamel and dentin in depth of color, contour, and light reﬂection,the ﬁnishing and polishing creates the illusion of reality. Factor in occlusion oand maintenance, and direct composite restorations are the most unique and thconservative restorations mirroring the reality of a tooth. AuReferences Lee SM. Preface. Dictionary of composite materials technology. Lancaster (PA): Techmic Publishing Company; 1989. Albers HF. Tooth colored restorations: principles and techniques. 9th edition. BC Decker Publishing; 2002. Craig R, Powers J. Restorative dental materials. Chapter 9. 11th edition. Mosby; 2002. Suh B. Update on adhesive dentistry. Presented at International Adhesive Symposium. Schaumburg (IL): Bisco, February 2007. Terry D. Application of nanotechnology. Editorial Commentary, Pract Periodontics Aes- thet Dent 2004;16(3):220–2.
AESTHETIC ANTERIOR COMPOSITE RESTORATIONS 377  Leinfelder KF, Sluder TB, Sockwell CL, et al. Clinical evaluation of composite resins as anterior and posterior restorative materials. J Prosthet Dent 1975;33(4):407–16.  Eubank J, LeSage B. Presented at the UCLA aesthetic continuum, composite lecture and hands-on workshops, 1997–2006. UCLA Dental School, Los Angeles.  O’Brien WJ, editor. Dental materials and their selection. 3rd edition. Carol Stream (IL): Quintessence Publishing Co; 2002. p. 114–6.  Mitra S, Wu D, Holmes B. An application of nanotechnology in advanced dental material. py J Am Dent Assoc 2003;134(10):1382–90. Sidaway I. Color mixing bible. NY: Watson-Guptill Publication; 2002. Dietschi D. Free-hand composite resin restorations: a key to anterior aesthetics. Pract Peri- odontics Aesthet Dent 1995;7(7):15–27. co Dietschi D, Dietschi JM. Current developments in composite materials and techniques. Pract Periodontics Aesthet Dent 1996;8:603–14. Dietschi D. Free-hand bonding in the esthetic treatment of anterior teeth: creating the illu- sion. J Esthet Dent 1997;9(4):156–64. Dietschi D, Ardu S, Krejci I. Exploring the layering concepts for anterior teeth. In: Rouley JF, Degrange M, editors. Adhesion: the silent revolution in dentistry. Chicago: Quintes- al sence; 2000. p. 235–51. Chiche G, Pinault A. Aesthetic of anterior ﬁxed prosthodontics. Chicago: Quintessence; 1994. on Dietschi D. Layering concepts in anterior composite restorations. J Adhes Dent 2001;3: 71–80. Gordon AA, vonderLehr WN, Herrin HK. Bond strength of composite to composite and bond strength of composite to glass ionomer lining cements. Gen Dent 1986;34: rs 290–3. Terry D, Leinfelder K. An integration of composite resin with natural tooth structure: the CL IV restoration. Pract Proced Aesthet Dent 2004;16(3):235–42. pe Miller M. Reality: the information source for esthetic dentistry. Houston (TX): Reality Publishing; 2006. Fahl NJ. Predictable aesthetic reconstruction of fractured anterior teeth with composite resins: a case report. Pract Periodontics Aesthet Dent 1996;8(1):17–30. Devoto W. Clinical procedure for producing aesthetic stratiﬁed composite resin restorations. Pract Proced Aesthet Dent 2002;14(7):541–3. rs Sproul RC. Color matching in dentistry. Part 1. The three-dimensional nature of color. J Prosthet Dent 2001;86:453–7. Hall NR, Kafalias MC. Composite colour matching: the development and evaluation of a restorative colour matching system. Aust Prosthodont J 1991;5:47–52. o Vanini L. Light and color in anterior composite restorations. Pract Periodontics Aesthet th Dent 1996;8(7):673–82. Deliperi S, Bardwell DN, Congiu MD. Reconstruction of severely damaged endodontically treated and bleached teeth using a microhybrid composite resin: two-year case report. Pract Au Proced Aesthet Dent 2003;15(3):221–6. Vanini L, Mangani FM. Determination and communication of color using the ﬁve color dimensions of teeth. Pract Proced Aesthet Dent 2001;13(1):19–26. Behle C. Placement of direct composite veneers utilizing a silicone build-up guide and intrao- ral mock-up. Pract Periodontics Aesthet Dent 2001;12(3):259–66. Jeﬀeries SR, Barkmerier WW, Gwinnett AJ. Three composite ﬁnishing systems: a multisite in vitro evaluation. J Esthet Dent 1992;4(6):181–5. Goldstein RE. Finishing of composite and laminates. Dent Clin North Am 1999;33(2): 305–18. Miller M. Contouring and polishing resin-based materials. Reality; the techniques. 2003;1:23–29.
378 LESAGE Powers JM, Fan PL, Raptis CN. Color stability of new composite restorative materials under accelerated aging. J Dent Res 1980;59(12):2071–4. Sarac D, Sarac SY, Kulunk S. The eﬀects of polishing techniques on the surface roughness and color change of composite resins. J Prosthet Dent 2006;96:33–40. Blitz N. Diagnosis and treatment evaluation in cosmetic dentistry: a guide to accreditation criteria. American Academy of Cosmetic Dentistry; Madison (WI). py co al on rs pe o rs th Au